Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses


 Emmeline Baldwin
 1 years ago
 Views:
Transcription
1 International Journal of Adhesion & Adhesives 20 (1999) International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses John A. Nairn Department of Material Science and Engineering, University of Utah, 122 S. Central Campus Drive, Room 304 Salt Lake City, UT , USA Received 6 November 1996 Abstract The mode I energy release rate, including the effect of residual stresses, was evaluated for both adhesive and laminate double cantilever beam specimens. The energy release rate can be partitioned into a mechanical term and a residual stress term in beam theory. The beamtheory mechanical term is not very accurate, but can be corrected by a slight modification to a previous correction factor. This correction factor accounts for crack tip rotation of the specimen arms. The beamtheory residual stress term is very accurate for a wide range of specimen geometries; it can be used without correction. The consequence of ignoring residual stresses is that one measures an apparent toughness instead of a true toughness. The error between the apparent toughness and true toughness can be calculated for a given specimen geometry and amount of residual stresses. Such errors can be large and are often larger than the correction required for cracktip rotation effects. In double cantilever beam specimens used to study laminate delamination, the errors are large when the delaminating arms, considered by themselves, are unsymmetric laminates. Some experimental methods are suggested which can used to correct for residual stress effects. Keywords: Adhesive Toughness, Fracture Mechanics, Residual Stresses, Delamination 1. Introduction Since the work of Mostovoy, Ripling, et al. [1 3], the double cantilever beam (DCB) specimen geometry has been a popular method for measuring the fracture toughness of adhesive bonds and delamination fracture toughness of composite laminates. There are existing standard protocols for mode I testing of both adhesive bonds [4] and laminate delamination [5]. The same specimen geometry with modified loading methods can be used for the study of mode II and mixed mode fracture as well [6, 7]. There are ongoing efforts to refine adhesive fracture and delamination methods to give the best possible results [8]. These standards, however, do not address methods for dealing with residual stresses. When adhesive joints are cured, or laminates are processed, at high temperature and then cooled to room temperature, residual stresses will inevitably be present. These stresses can arise either from differential thermal shrinkage between the components of the specimen or from chemical shrinkage of the adhesive or composite matrix resins. When a crack grows in a specimen with residual stresses, the residual stresses can contribute to the total amount of energy released. If residual stress effects are ignored, the calculated fracture toughness will not be the true fracture toughness. Instead, it will be an apparent toughness that includes a specimen property (the amount of residual stresses) within the desired material property (the toughness). When such an apparent toughness is used for prediction of failure in adhesive joints that have different levels of residual stresses, those predictions will not be correct. Furthermore, the most common residual stress effect in adhesive DCB specimens is for Tel: ; fax: address: (J.A. Nairn) /00/$see front matter c 2000 Elsevier Science Ltd. All rights reserved.
2 60 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) the apparent toughness to be larger than the true toughness. Thus, adhesive designs based on such nonconservative apparent toughnesses could lead to premature failure. This paper describes a mode I energy release rate analysis for crack growth in adhesive DCB specimens and laminate delamination specimens. The thermoelastic energy release rate analysis uses linearelastic beam theory. Largedisplacement, endblock loading, and plasticity effects were ignored, but these effects could be included by methods developed previously for delamination [7, 9] and adhesive fracture [10] analysis. The crack is assumed to propagate straight; for adhesives, it is therefore assumed to remain in the middle of the adhesive as a cohesive mode I fracture. The energy release rate can be partitioned into two terms a term involving mechanical loads and a term involving residual stresses. The accuracy of each term was studied by extensive finite element calculations. As observed in previous work, the beamtheory mechanical term is inaccurate because it ignores arm rotation at the root of the crack [7, 10, 11]. A previouslypublished correction to the mechanical term [10] is very accurate, provided it is multiplied by a numericallydetermined constant. In contrast, the beamtheory residual stress term is accurate, without correction, for a wide range of specimen geometries. From the accurate residual stress term, it is possible to calculate the error induced in the measured fracture toughness for any DCB specimen, if residual stresses are ignored. The error in adhesive DCB specimens can be significant. It gets smaller as the adhesive layer gets thinner and as the modulus ratio between the adherend and the adhesive gets larger. In laminate DCB specimens, the residual effect disappears if both arms of the DCB specimen are themselves symmetric laminates. If the arms are not symmetric laminates, the residual stress effect will generally be significant. Finally, accounting for residual stresses in analysis of DCB specimens requires knowledge of the level of residual stresses in the specimen. Some experimental methods based on calibration specimens, on observing initial beam curvatures, or on the loaddisplacement curve are discussed. The recommended method is to extrapolate the residual stress term from a properlyzeroed, loaddisplacement curve. Although the energy release rate analysis is specific for residual thermal stresses, the experimental correction method is general; it can account for any type of residual stresses. 2. General energy release rate analysis Figure 1 shows a double cantilever beam (DCB) specimen geometry used to measure the mode I toughness of adhesive bonds. In a fracture mechanics analysis of this specimen, the crack is predicted to propagate when the thermoelastic energy release rate for mode I crack growth (G I ) becomes equal to the toughness of the adhesive or the adhesive s critical energy release rate (G ). The mechanics problem is thus to find G I including the effect of residual stresses. A recent paper [12] has derived an exact result for mode I energy release rate in any composite with residual stresses: G I = d Gmech + 1 da 2 σ m α T dv V Gmech 2 (1) where G mech is the energy release rate in the absence of residual stresses, σ m is the stress tensor due to mechanical loads only, α is the positiondependent thermal expansion tensor of the composite material, and T = T s T 0 is the temperature difference between specimen test temperature (T s ) and the stressfree temperature (T 0 ). The derivative in the numerator is with respect to total crack area A. In this analysis, the adhesive DCB specimen is treated as a twophase composite with the two phases being the adhesive joint and the two adherends. Equation (1) was derived using a linear thermoelasticity analysis. It assumes residual stresses arise due to differential thermal shrinkage between the phases of the specimen under a uniform change in temperature of T [12]. Some experimental methods to correct for other types of residual stresses are discussed below. For the tractiononly loading of the adhesive DCB specimen (see Figure 1), some further results from Ref. 12 are that G mech = 1 d T 0 u m ds and σ m α T = T 0 u r ds (2) 2 da S V S
3 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) P y x v m + v r Adherend Adhesive b a La P Fig. 1. A double cantilever beam specimen used to measure the mode I toughness of adhesive bonds. The cantilever arm length is a, the total specimen length in L. Sometimes the adhesive does not extend to the end of the arms; here the adhesive stops a distance b from the ends. where T 0 is the applied surface traction, u m and u r are the displacements due to mechanical or residual stresses, respectively. For a 2D, planestress analysis (all stresses in the z direction assumed to be zero), the tractions applied to the DCB specimen are T 0 = P B δ( x x u) P B δ( x x l) (3) where P is the total applied load, B is the specimen thickness in the z direction, δ( x) is the Dirac delta function, and x u and x l are the locations of the upper and lower loading points. Substitution of this traction vector into equations (1) and (2) with da = B da, where a is the DCB specimen arm length, leads to G I = G mech + P dv 2 r da Gmech and G mech = P B where v m and v r are the load point displacements at the top loading point ( x u ) in the y direction due to mechanical or residual stresses, respectively (see Figure 1). In general, residual stresses can contribute to energy release rate either by releasing strain energy or by doing external work as the crack grows [12]. The residual stress contribution to energy release rate here is the second term in equation (4). It is immediately seen to be equal to the external work caused by changes in residual displacements (v r ) under load P at the loading points. In other words, the entire effect of residual stresses in DCB specimens is an external work effect arising from thermally induced curvature in the DCB arms. Although the full DCB specimen is a balanced structure, each DCB arm is an unbalanced, twolayer structure. As the crack grows, the unbalanced arms may curve due to residual stresses; this curvature leads to external work that causes the entire residual stress effect in G I. By equation (4), the analysis for G I is reduced to finding the loading point mechanical and residual displacements. Here one arm of the specimen will be analyzed by simple beam theory. We begin by writing the upperarm, momentcurvaturetemperature relation as dv m da κ = d2 v dx 2 = C κm + α κ T (5) where κ is beam curvature (defined as positive for curvature upwards), v is ydirection displacement, M is the applied moment, C κ is the effective beam bending compliance, and α κ is the effective beam thermalcurvature coefficient. In common adhesive specimens, the adhesive joint does not extend all the way to the loading point as shown in Figure 1 where the adhesive stops at a distance b from the end. An analysis for finding beam displacements must account for the different values of C κ and α κ in the region with adhesive and the region with no adhesive. Because b remains constant, however, as the crack propagates, the beam (4)
4 62 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) section with no adhesive makes a constant contribution to displacements that drops out when derivatives with respect to a are evaluated. In other words, G I is independent of b; for simplicity we can evaluate loadpoint displacements by setting b = 0. Integration of equation (5) for mechanical stresses only (M = P x, T = 0, and x = 0 at the loading point) or residual stresses only (M = 0, T 0) leads to where v m = 1 3 C κp a 3 and v r = 1 2 α κ T a 2 (6) Substituting loadingpoint mechanical and residual displacements into equation (4) gives C m = G I = (C m P a + C r T ) 2 (7) C κ B and C r = α κ C κ B The G I analysis has been reduced to the problem of finding the effective beam properties of the cantilever arms. Specific results for adhesive or laminate DCB specimens are given in the following two sections. In many adhesive DCB specimens, such as those with polymeric adhesives and metallic adherends, α κ T, and hence v r, will be negative. This fact seems to invalidate the residual displacement analysis because it corresponds to the upper arm displacing down and through the lower arm. The G I analysis, however, remains valid provided the total beam displacement, v = v m + v r, is positive; in other words, the analysis remains valid for any adhesive DCB test where the beam arms must be mechanically opened to induce fracture. The situation where the crack grows without v being positive corresponds to a specimen that fails due to residual stresses alone and therefore to a specimen that would not be used in a subsequent adhesive fracture test. (8) 3. Adhesive double cantilever beam specimens Analysis of adhesive DCB specimens was reduced above to finding the effective beam properties, C κ and α κ, both of which can be found by simple composite beam analyses. The preferred, but still simple, analysis is one that considers the full beam geometry or one that does not assume the adhesive is thin. The coordinates for analysis of one adhesive DCB arm are shown in Figure 2. By simple beam analysis (e.g., Ref. 13) C κ = 1 1 = (9) (EI) effective E 1 I zz,1 + E 2 I zz,2 where E i and I zz,i are the modulus and moment of inertia about the neutral axis for phase i (i = 1 for the adherend and i = 2 for the adhesive). The neutral axis is located at y N = h 1h 2 2 E 1 E 2 E 1 h 1 + E 2 h 2 (10) where h 1 and h 2 are the thicknesses of the adherend and adhesive, respectively. By the parallel axis theorem ( I zz,1 = Bh Bh 1 y N h ) 2 ( 2 and I zz,2 = Bh Bh 2 y N + h ) 2 1 (11) 2 The beam C κ can be written in a convenient form as C κ = 12 E 1 Bh 3 1 λ 2 (1 + Rλ) ( 3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ 1 ) (12) where R = E 1 E 2 and λ = h 1 h 2 (13)
5 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) h/2 B y h 1 E 1 x h/2 h 2 E 2 Fig. 2. The coordinate system used for composite beam analysis of one arm of an adhesive DCB specimen. The result for α κ is the classic Timoshenko, bimetallic strip problem [14] which can be written as ακ 6 α(1 + λ) = ( h 2 (3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ 1 )) (14) where α = α 1 α 2 is the difference in thermal expansion coefficients between the adherend and the adhesive. For typical polymeric adhesives with metallic adherends, α 1 < α 2 and T < 0 as the specimen cools from the cure temperatures to the testing temperature. For such specimens, ακ T < 0, and the residual stresses cause the beam arms to bend towards the center of the specimen. Thus, in such specimens, the residual stresses cause the beam arms to do work on the loading system. From equation (8), the mechanical and residual coefficients for determining G I are C m = 2λ 3(1 + Rλ) Bh 1 E 1 h 1 (3(1 + λ) 2 + (1 + Rλ) C r = 3E 1 h 1 α(1 + λ) ( (1 + Rλ) 3(1 + λ) 2 + (1 + Rλ) 3.1. Comparison to finite element results ( λ 2 + Rλ 1 )) (15) ( λ 2 + Rλ 1 )) (16) For judgement of the accuracy of C m and C r, a large number of finite element calculations (FEA) were done in which R was varied from 1 to 100 and λ was varied from 1 to 128. The accuracy of beam theory depends on the axial ratio of the beam arms; thus for each pair of R and λ, analyses were done for arm axial ratios (a/h) from 2.5 to 160. For these calculations, the adhesive properties were held constant at E 2 = 2500 MPa, ν 2 = 0.35, and α 2 = K 1 ; the adherend modulus was E 1 = RE 2 while ν 1 = 0.3 and α 1 = K 1 were held constant. The arm geometry (see Figures 1 and 2) was set to h = 5 mm and L = 2a = 2h(a/h); the analysis is independent of B. The composite beam was meshed into 8noded, isoparametric, quadrilateral elements with midside nodes. The energy release rate, G I, was calculated by crack closure methods [15]. With square cracktip elements, it was possible to get accurate results even with relatively coarse meshes. All results reported here were for a sufficiently refined mesh of about 600 elements and 2000 nodes. As expected, the errors in beamtheory C m and C r got larger as the arm axial ratio got smaller. At constant a/h, however, the relative errors in C m and C r were approximately independent of R and λ. The absolute value of the errors in C m or C r, averaged for λ from 1 to 128, are plotted as a function of a/h in Figure 3. Figure 3 is for R = 28 which corresponds to aluminum adherends (E 1 = MPa) with a typical epoxy adhesive (E 2 = 2500 MPa). The results for any other value of R (from 1 to 100) were similar, except that the errors for small a/h grew slightly at larger values of R. The errors in the residual stress coefficient, C r, were always less than 1% for a/h > 5 and were typically less than 0.01% for a/h > 10. For a/h < 5, the errors were still low for R < 20, but got larger and depended on λ for R > 20. Thus, except for the combination of a/h < 5 and R > 20, the simple beam theory result for C r does an excellent job of evaluating the contribution of residual stresses to total energy release rate.
6 64 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) Coefficient Error (%) C m Error C r Error Arm Axial Ratio (a/h) Fig. 3. The average or the absolute values of the errors between the theoretical coefficients C m and C r and the mechanical and residual stress results calculated by FEA as a function of the arm axial ratio. These results are for R = 28. For each arm axial ratio, the error was averaged for λ from 1 to 128. Because typical adhesive DCB specimens strive to use long, slender arms (large a/h), the residual stress correction evaluated here should be sufficiently accurate for all commonlyused adhesive fracture specimens. The errors in C m normally exceeded 1% and got very large for small a/h. This observed error in simple beam theory for calculating mechanical energy release rate has been discussed before [7 10]. The error is caused by an oversimplification in the simple beam theory analysis that prevents rotation of the specimen arms at the crack tip; for accurate analysis, this rotation can not be ignored. Williams analyzed an adhesive DCB specimen ignoring residual stresses [10]. He wrote a corrected mechanical beam theory result as G I ( T = 0) = (C m (a + W ) P ) 2 where C m = lim λ C m = 12 EB 2 h 3 1 is the limiting mechanical energy release rate coefficient for a very thin adhesive. In other words, the corrected analysis replaces the true crack length, a, by an effective crack length, a + W. Using the beamonelasticfoundation model of Kanninen [16], Williams derived the effective crack length correction in terms of specimen properties to be ( ) 1/4 1 + R λ W = h 1 (18) 6 If G F I EA is the energy release rate calculated by finite element analysis with T = 0, a numericallydetermined effective crack length correction for equation (17) can be found from F EA = (17) G F EA I C m P a (19) When including specimens with possibly thick adhesive layers, however, it is preferable to find the effective crack length correction relative to the full composite beam analysis for C m rather then for the thinadhesive beam result of C m. In other words, here the FEA effective crack length correction was found from F EA = G F EA I C m P a (20)
7 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) When this numericallycalculated F EA was compared to the theoretical W in equation (18) for all finite element calculations, they were found to be related by an almost constant ratio of F EA W = 1.15 (21) This ratio was independent of λ (in the range of 1 to 128) and a/h (in the range 2.5 to 160). The ratio was weakly dependent on R it was independent of R for R > 5 and increased slightly at low R, reaching 1.20 when R = 1. No attempt was made to derive the origin of the constant ratio of F EA to W. The beamonelastic foundation analysis in Ref. 10 ignored shear stresses although it was noted they could be added using the methods of Ref. 11. Because shear corrections depend on beam axial ratio while the results here were independent of arm axial ratio, it is unlikely that shear effects account for the discrepancy. Simple beam theory is one dimensional and thus does not account for Poisson ratio mismatch effects. To test for an effect of ν 1 ν 2 on the correction ratio, some additional calculations were done for R = 28 and ν 1 varying from to Again, there was no effect on the F EA / W ratio. The numerical result of 1.15 W can thus be regarded as a numericallydetermined correction factor valid for any typical adhesive DCB specimen with isotropic layers. Using the numericallydetermined adjustment to W, the energy release rate can be written as G I = ( (C m ) ) 2 W P a + C r T (22) a The average errors for all values of a/h 2.5 were less than 1% and typically much less than 1%. The maximum errors in the mechanical term occurred for small R while the maximum errors in the residual stress term occurred for large R. Even these maximum errors, however, were smaller than 1%, provided a/h Consequence of ignoring residual stresses Many previous adhesive toughness experiments have ignored residual stresses. The energy release rate result in equation (22) can be used to calculate the errors of such an approach. Assume that some particular adhesive has a true fracture toughness of G. If an adhesive DCB specimen with this adhesive is tested, it will fail when G I = G, which occurs when P = G C r T C m (a W ) (23) Notice that P < 0 if G < Cr 2 T 2. This condition corresponds to a DCB specimen that fails due to residual stresses alone. If the observed failure load is then used in an analysis that ignores residual stresses (equation (22) with T = 0), the apparent toughness and its percent error relative to the true G would be [ ( ) ( 2 G app = G C r T and G app Error = C ) ] 2 r T 1 (24) G This error, or consequence of ignoring residual stresses, can be calculated without knowledge of C m or W. For a sample calculation of errors due to ignoring residual stresses, we considered an adhesive with G = 200 J/m 2 and residual stresses due to α = K 1 and T = 100 C. These parameters correspond to a typical hightemperature cure epoxy adhesive bonded to metallic adherends. The total differential strain of α T = 0.40% is not excessively large for adhesive specimens. Because C r T < 0, G app will be higher than the true toughness. Figure 4 plots the percentage error in G app as a function of R for various λ from 2 to 64. The errors are extremely large for low R and low λ and decrease as either R or λ increase. In general, the errors are never insignificant. The dashed vertical line shows a typical R value for aluminumepoxy specimens (R = 28). Despite the high aluminumepoxy R value, the errors exceed 1% even with a very thin adhesive (λ = 64). The errors in aluminumepoxy specimens increase to over 40% as λ decreases to 2. Finally, the errors depend on total arm thickness (h). The results in Figure 4 were for h = 5 mm; the errors increase for specimens with larger h.
8 66 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) λ = 2 35 app G Error (%) λ = 8 λ = 4 C m Error (a/h=20) 15 λ = λ = 32 λ = Moduls Ratio (R = E 1 /E 2 ) Fig. 4. The error in G app when residual stresses are ignored as a function of R for various values of λ. The adhesive DCB specimens were assumed to have h = 5 mm, G = 200 J/m 2, α = K 1, and T = 100 C. The vertical dashed line corresponds to R = 28 which is a typical value for aluminumepoxy specimens. The nearlyhorizontal dashed line gives the errors caused in the mechanical energy release rate when ignoring the cracklength correction term for beam arms with a/h = 20. Early work on adhesive fracture using DCB specimens investigated the effects of adhesive joint thickness, DCB specimen width, and postcure temperature [1 3] on toughness, but these experiments ignored residual stresses and thus actually observed changes in G app instead of the true G. Interestingly, all experimentally observed trends in G app match predicted trends if we assume all changes are due solely to a change in level of residual stresses. As the adhesive joint gets thicker, λ get smaller which increases the residual stress effect and causes G app to increase; this prediction matches experiments [2, 3]. As the DCB specimen width changes, there should be no effect on G app ; this prediction matches experiments [3]. As the postcure temperature increases, T gets more negative, which increases the residual stresses and causes G app to increase; this prediction matches experiments [2, 3]. The magnitude of the observed G app changes with joint thickness and postcure temperature [2, 3] are probably larger than can be accounted for by a residual stress effect alone. It is likely, however, that residual stresses account for a nonnegligible fraction of the changes. The most appropriate physical picture of the changes in toughness should be derived from the true G instead of from G app. In one paper on postcure temperature effects, Mostovoy and Ripling [2] concluded that residual stresses are not important because G app increased with postcure temperature while they expected that an increased level of residual stress could only cause G app to decrease. This assessment is incorrect; in typical polymeric adhesives with metallic adherends, increasing the level of residual stresses causes G app to increase. Much effort has gone into corrections to the beamtheory mechanical term in proposing standards for mode I fracture of adhesive specimens [8, 10]. It is therefore interesting to compare the magnitude of the errors induced by ignoring the mechanical correction to those induced by ignoring residual stresses. If we consider a specimen with no residual stresses and a true toughness of G, by a similar procedure applied to analysis of residual stress errors, the percent error in the apparent toughness with respect to the true toughness caused by ignoring the mechanical term correction factor is [ ( ) 2 G app a Mechanical Error = 100 1] (25) a W This error is nearly independent of λ, but is a strong function of a/h and a weak function of R. Superimposed on Figure 4 is the mechanical error of typical adhesive specimens with a/h = 20. For an aluminum/epoxy specimen (R = 28), the residual stress error is larger than the mechanical error for thicker adhesives (λ < 10), but gets smaller for thinner adhesives (λ > 10). As a/h gets larger, the mechanical errors get smaller while
9 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) the residual stress errors do not change. Thus, for larger a/h, the residual stress errors will usually be larger than the mechanical errors. The exact value of the residual stress error depends on specimen geometry and the level of residual stresses in the adhesive, but in ordinary adhesive specimens it will often have a magnitude similar to the error induced by ignoring crack tip rotation. It makes little sense to carefully correct for all mechanical effects while ignoring a similarmagnitude residualstress error, especially since the residual stress effect can be accurately included by use of the C r T term in the energy release rate expression in equation (22) Asymptotic results for thin adhesives Many analyses of adhesive specimens assume the adhesive is thin. To judge the conditions for which the thinadhesive limit is valid, we derived asymptotic expansions for C m, C r, and W and compared those results to the full composite beam results. Expanding all results in a Taylor series in 1/λ and truncating after the linear terms gives the following asymptotic results: ( 12 C m (λ large) = E 1 B 2 h ) + O[1/λ 2 ] (26) 1 2Rλ C r (λ large) = α 3E1 h 1 + O[1/λ 2 ] (27) Rλ W (λ large) = h 1 ( 1 + R 4λ ) + O[1/λ 2 ] (28) The constant term in each limiting expression is the result as λ : Cm = lim C 12 m = λ E 1 B 2 h 3, Cr = lim C r = 0, and W = lim W = h 1 (29) 1 λ λ Notice that in the limit of no adhesive, there will be no beam curvature due to mismatched thermal expansion coefficients and thus the residual stress effect vanishes (Cr = 0). Figure 5 plots C m (λ large), Cm, C r (λ large), W (λ large), and W as a function of λ for a typical aluminumepoxy specimen. Each limiting result has been normalized to the full composite beam results in equations (15), (16), and (18) and thus deviations from 1 give the error caused by use of a limiting result rather than the full result. The limiting result Cr is not plotted because it is always zero. Both C m (λ large) and Cm converge very rapidly and agree within 1% with the full beam analysis, provided λ > 10. All other constants converge more slowly. C r (λ large) and W (λ large) require λ > 80 to be within 1% of the full beam analysis while W requires λ > 700. Figure 5 is for R = 28. The C m results converge faster as R gets larger while the W results converge slower. The C r convergence is relatively insensitive to R. In summary, it is acceptable to use thinadhesive, asymptotic results for C m, provided λ is larger than about 10 and R is not too small. For typical adhesive DCB specimens, however, it is not accurate to use the thinadhesive limits for either C r or W. The full expressions in equations (16) and (18) should be used instead. In other words, the fact that Cr = 0 or C r (λ large) is small does not imply that residual stresses can be ignored for thin adhesives Experimental suggestions By using equation (22) with C r determined by equation (16), it is possible to accurately determine G I for any typical adhesive DCB specimen including the effect of residual stresses. There are two experimental problems when correcting for residual stresses. First, evaluation of C r requires knowledge of α and T. Second, even if α and T are known, the form of C r in equation (16) assumes that both the adhesive and adherend are linear thermoelastic materials with temperatureindependent thermomechanical properties between T 0 and T s and that residual stresses are caused solely by differential thermal shrinkage. In real specimens, the thermomechanical properties will probably depend on temperature (especially in the adhesive near T 0 ) and there may be additional sources of residual stresses such as chemical shrinkage during adhesive cure. This section suggests some experimental methods for accounting for residual stresses that will be valid for any form of residual stresses.
10 68 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) W (λ large) Limiting Term/Full Term C m C m (λ large) W C r (λ large) λ Fig. 5. Plots of C m (λ large), C m, C r (λ large), W (λ large), and W as a function of λ. Each constant has been normalized the the full beam analysis results (C m, C r, and W ). These plots are for an aluminumepoxy specimen with R = 28 and h = 5 mm. By equation (5), each arm of the adhesive DCB specimen is assumed to have an effective momentcurvature relation. In the absence of mechanical loads, the curvature due to residual stresses is κ res = α κ T (30) To account for any type of residual stresses, we simply repeat the previous analysis but use κ res to calculate residual stress effects instead of α κ T. The result is that equations (7) and (8) change to where C res = κ res C κ B = κ resh 1 E 1 h 1 2λ 3 G I = (C m P a + C res ) 2 (31) ( 3(1 + λ) 2 + (1 + Rλ) λ 2 + Rλ Rλ The problem of accounting for residual stresses is reduced to experimentally finding κ res ; some possible experimental methods are illustrated in Figure 6. The method in Figure 6A is to construct a calibration specimen for each adhesive DCB specimen and subject it to identical adhesive cure conditions. The calibration specimen is a twolayer, adhesive and adherend strip. Such an unbalanced structure will curve due to residual stresses. By measuring the chord length, l, and strip height, d, the residual stress curvature can be calculated from [17] κ res = 2d (33) d 2 + l2 4 The sign of κ res is determined by the direction of curvature κ res is negative if the strip curves toward the adhesive and positive if it curves toward the adherend. Two drawbacks of using calibration specimens are that it requires preparing an extra specimen for each adhesive DCB specimen and that it may not be possible to subject the calibration specimens to identical cure conditions. Even when subjected to the same thermal history, the lack of an adherend on both sides of the adhesive may cause the calibration specimen to develop different residual stresses than the adhesive DCB specimen. Prior to a test, the arms of an adhesive DCB specimen with residual stresses will have some initial curvature caused by those stresses. Figures 6B and 6C show the possible types of initial arm curvature. This initial curvature could be used to determine κ res. This approach avoids the need for contruction of a ) (32)
11 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) l d A B C δ 0 δ 0 P D E h 2 δ int δ 2h 2 h 2 0 Fig. 6. Some experimental methods for determining the effect of residual stresses on G I in adhesive DCB specimens. A. Measure the curvature of an unbalanced, twolayer, adhesive and adherend strip. B. Measure initial arm curvature when κ res > 0. C. Measure initial arm curvature when κ res < 0. D. Determine intercept in loaddisplacement curve. E. Prepare symmetric specimens. second calibration specimen and guarantees that κ res is measured from the correct cure conditions. Figure 6B corresponds to a specimen with κ res > 0. For such specimens the arms will separate. From equation (6), the initial, total beam opening, δ 0, is related to κ res by δ 0 = a 2 κ res or κ res = δ 0 a 2 (34) Figure 6C corresponds to a specimen with κ res < 0. For such specimens, the arms will bend towards each other, but the arm ends will contact each other, inducing a load that prevents interpenetration. Integration of equation (5) and evaluation of the load P (M = P x) required for zero displacement at x = 0 shows that the maximum arm separation occurs at x = a/3. The maximum separation, δ 0, is related to κ res by δ 0 = 2a2 κ res 27 or κ res = 27δ 0 2a 2 (35) Notice that for specimens with identical magnitudes of κ res, the maximum arm separation used for determination of κ res is more than an order of magnitude smaller when κ res < 0 than it is when κ res > 0. This observation has two consequences. First, it may be difficult to accurately measure κ res when it is negative; this drawback is particularly troublesome because κ res is negative for most adhesive specimens. Second, an observation that there is not much initial curvature in the arms of an adhesive DCB specimen with κ res < 0 is not sufficient justification for ignoring residual stresses in that specimen. Perhaps a better way to measure κ res from the adhesive DCB specimen itself is to extract it from a measured loaddisplacement curve. Figure 6D shows an expected loaddisplacement curve where the displacement is the total arm displacement between the bottom surfaces of the arms measured at the loading points (x = 0). This curve is for an adhesive specimen with negative κ res ; the nonzero load at zero displacement is the load induced that prevents arm penetration. By extrapolation of the linear loaddisplacement curve with positive displacements to zero load, it is easy to show that the intercept, δ int, is related to κ res by δ int = a 2 κ res or κ res = δ int a 2 (36)
12 70 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) y 1 y 2 +h/2 h 1 h 2 E 1, α 1, θ 1 E 2, α 2, θ 2 B y x y n h/2 h n E n, α n, θ n Fig. 7. The coordinate system used for laminated beam analysis of one arm of an laminate DCB delamination specimen. The extrapolation methods works equally when for κ res > 0 and κ res < 0. The only difference is that when κ res < 0, the extrapolation must be done from positive displacements, which can be measured, into negative displacements, which cannot be measured. The only drawback of this interceptextrapolation method is that it requires the extra effort of accurately measuring beam opening during the experiments. The measured displacement must also be accurately calibrated to give zero displacement when the beam arms touch. Many adhesive specimens have an adhesive dropoff before the end of the specimen, as illustrated by the zone of length b in Figure 1. The extrapolation method can be modified to handle such specimens. Integration of the beam momentcurvature relation with allowance for a change in beam properties at x = b gives the intercept of the load displacement curve as δ int = 2h 2 + (a 2 b 2 )κ res or κ res = δ int 2h 2 a 2 b 2 (37) Here 2h 2 is the additional beam opening at the loading point because there is no adhesive present and the (a 2 b 2 ) term corrects for the reduced length of the zone with adhesive. When κ res < 0, the extrapolation must be made from displacements greater than 2h 2. The final experimental suggestion for dealing with residual stresses is to prepare specimens with no residual stress effect. As explained above, the entire effect of residual stresses can be traced to external work done by the arms as they curve due to the presence of residual stresses. This curvature can be eliminated by constructing symmetric DCB arms. As shown in Figure 6E, symmetric arms can be made by adding a layer of adhesive of thickness h 2 to both the top and bottom surfaces of the adhesive DCB specimen. The residual stresses can be ignored in the analysis of such a specimen. Three drawbacks of symmetric arms are that they complicate specimen fabrication, that the thickness of the outer layers must be carefully controlled to h 2 (or half to total adhesive joint thickness), and that the cure conditions must guarantee that the adhesive on the surfaces develop an identical level of residual stresses as the adhesive joint. 4. Laminate double cantilever beam specimens Another application of double cantilever beam specimens is to measure mode I delamination toughness of composite laminates [5]. By starting from equations (7) and (8), solving the laminate problem for energy release rate including the effect of residual stresses is simply a matter of determining Cκ and ακ for each arm of the laminate specimen. A simple laminated beam analysis of the single DCB arm in Figure 7 is given in the Appendix; substituting those results for Cκ and ακ into equation (8) gives the required C m and C r needed to for total G I. This planestress, laminate analysis treats the composite arms as beams. It therefore ignores possible anticlastic curvature and bendingtwisting coupling effects [18, 19]. As with adhesive DCB specimens, the simple beam theory result for C m is not very accurate and needs to be corrected for beam rotation effects. As with the adhesive DCB specimen, that correction can be done by introducing an effective crack length as has been discussed by Williams [11]. Because laminate DCB arms are orthotropic materials, the C m correction differs from the one for adhesive DCB specimen with isotropic arms [11]. The remainder of this section will only consider the effects of residual stresses and suggest experimental methods for accounting for residual stresses. Each of these topics can be analyzed accurately without knowledge of the correction factors required for C m.
13 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) Table 1. Errors caused by ignoring residual stresses in delamination experiments on a series of graphite/epoxy laminates. The experiments are assumed to be on 16ply laminates with delamination in the middle of the laminate. The laminates listed here are the layups for the 8ply laminates in each DCB specimens. 8Ply Arm G IC Error 8Ply Arm Layup G IC Error (%) Layup (%) [0 8 ] 0.00 [0 2 /90 2 /0 2 /90 2 ] [90/0 7 ] [0/90/0/90/0/90/0/90] [90 2 /0 6 ] [90/0/90/0/90/0/90/0] [90 4 /0 4 ] [90 2 /0 2 /90 2 /0 2 ] [90 6 /0 2 ] [0 2 /90 2 /45 2 / 45 2 ] [90 8 ] 0.00 [90 2 /0 2 /45 2 / 45 2 ] [0 2 /90 6 ] [0 2 /45 2 / 45 2 /90 2 ] [0 4 /90 4 ] [90 2 /45 2 / 45 2 /0 2 ] [0 6 /90 2 ] [45 2 / 45 2 /0 2 /90 2 ] [0 7 /90] [ 45 2 /45 2 /90 2 /0 2 ] Consequence of ignoring residual stresses From equation (24), the error caused by ignoring residual stresses is a function only of C r, T, and G IC. We considered a series of graphite/epoxy laminates with G IC = 200 J/m 2 and T = 125 C, which are typical values for graphite epoxy laminates [20 22]. The value of C r depends on the layup of the specimen arms and can be calculated by the laminated beam analysis in the Appendix followed by substitution into equation (8). Table 1 lists the error caused by ignoring residual stresses for delamination down the middle of a series of 16ply laminates which leads to 8ply laminate DCB arms. In all examples, the undelaminated 16 ply laminate is symmetric; the 8ply arms, however, may be unsymmetric. The ply properties used in these calculations were E 1 = MPa, E 2 = 8970 MPa, ν 12 = 0.30, G 12 = 6900 MPa, α 1 = K 1, α 2 = K 1, and h i = mm. The first column of Table 1 gives a series of DCB arms with 0 and 90 plies. The two special cases of [0 8 ] and [90 8 ] are not affected by residual stresses and thus introduce no error. The arms in these specimens are themselves symmetric laminates and therefore do not curve due to residual stresses. Because there is no thermal curvature, there is no external work due to residual stresses and no residual stress effect on G I. These layups will have residual stresses caused by differential shrinkage between the fibers and the matrix. These residual stresses, however, do not release any energy as the delamination crack propagates. Many previous delamination experiments have been done on unidirectional laminates. It is correct to ignore residual stresses when analyzing such experiments. All other arrangements of 0 and 90 plies, besides [0 8 ] and [90 8 ], have an effect of residual stresses that cannot be ignored. The smallest error, caused by a change of a single ply on the surface, is 6.21% ([90/0 7 ]); the largest error is 76.36% ([0 2 /90 6 ]). An interesting example is the [0 4 /90 4 ] laminate. If the delamination growth is parallel to the fibers in the surface plies, the apparent G IC will be 46.54% too high (293 J/m 2 in this example). But, if the laminate is rotated 90 and the delamination is propagated parallel to the fibers in the central plies, the apparent G IC will be 37.68% too low (125 J/m 2 in this example). The two apparent toughnesses will differ by more than a factor of two. The second column of Table 1 lists some alternate layups with four 0 and four 90 plies and lists some quasiisotropic layups. Among the 0/90 laminates, the sign of the error depends on the stacking sequence and the magnitude depends on the ply groupings. Positive errors result when the 90 plies are in the middle while negative errors result when 0 plies are in the middle. The errors get smaller as the ply groupings get smaller; the smallest error is for alternating 0 and 90 plies. Among the quasiisotropic layups, the error ranges from % to %. It is not possible to construct laminate arms made from 0 2, 90 2, 45 2, and 45 2 ply pairs having a residual stress effect that causes less than a 14% error. If the ply pairs are split apart, the errors can be made smaller. Symmetric arm layups such as [0/90/ + 45/ 45/ 45/ + 45/90/0]
14 72 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) would have no residual stress effects Experimental suggestions Rather than calculate C r from laminated plate or beam theory and knowledge of T, it is preferable to experimentally correct for residual stresses. As with adhesive DCB specimens, experimental correction avoids having to measure additional thermomechanical properties and furthermore can account for residual stresses caused by any mechanisms. As with adhesive DCB specimens, residual stress curvature in laminate DCB specimens can be evaluated by using calibration specimens (Figure 6A), by measuring initial arm curvature (Figures 6B and 6C), or by extrapolating from carefullyzeroed, loaddisplacement results (Figure 6D). The extrapolation method is probably the best method. Also like adhesive DCB specimens, the residual stress effect can be eliminated by use of specimens with symmetric arms [18, 19] (Figure 6E). This approach is more attractive in delamination specimens than in adhesive specimens because instead of the extra work of adding layers and carefully controlling their thickness, it only requires selecting specimens with a doublysymmetric layup. Here, a doublesymmetric layup is a symmetric laminate for which each delaminating arm is itself a symmetric laminate. The absence of a residual stress effect in doublysymmetric laminates assumes the laminate was cooled slow enough such that there are no residual stresses due to thermal gradients during cooling. A specimen that is cooled rapidly would probably develop compressive stresses on the surface and tensile stresses in the middle. Such a distribution of residual stresses would cause the arms to curve away from each other as they delaminate or act like a specimen with κ res > 0 and give an apparent toughness that is lower than the true toughness. Because thermal gradient effects become larger as the laminate gets thicker, compression on the outside and tension in the middle would cause the toughness to decrease as the specimens get thicker. Because the axial thermal expansion coefficient of many unidirectional carbonfiber laminates is negative, an opposite situation would occur for delamination parallel to the fibers. Rapid cooling would cause tension on the outside and compression in the middle and the apparent toughness would increase as the specimens got thicker. Indeed, the apparent toughness of unidirectional IM6 carbon fiber/peek specimens has been observed to increase with arm thickness [23]. This observation, however, was attributed to fiber bridging instead of residual stresses [23]. That conclusion is supported by the extra experiments in Ref. 23 that showed that the toughness did not change as the cooling rate increased. Acknowledgements This work was supported by a grant from the Mechanics of Materials program at the National Science Foundation CMS Appendix A The effective properties of a laminate DCB specimen can be determined from laminated plate theory. Here, however, all analyses are planestress, beam analyses and therefore a laminated beam theory was used. For the laminate arm illustrated in Figure 7 under axial strain ε 0 and curvature κ, the axial strain as a function of y is ε(y) = ε 0 κy (38) where κ > 0 corresponds to curvature upward. The axial stress in each layer, including residual stresses, is σ(y) = E(y) ( ε 0 κy α(y) T ) (39) where E(y) and α(y) are the positiondependent modulus and thermal expansion coefficient in the x direction. Integrating these stresses, the total axial force, F, and bending moment, M, can be written as F = A 11 ε 0 B 11 κ N T T and M = B 11 ε 0 + D 11 κ + M T T (40)
15 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) where h/2 A 11 = B E(y)dy = B h/2 h/2 B 11 = B y E(y)dy = B h/2 n E(θ i )h i (41) i=1 h/2 D 11 = B y 2 E(y)dy = B h/2 n E(θ i )h i ȳ i (42) i=1 h/2 N T = B E(y)α(y)dy = B h/2 n ( ) E(θ i )h i ȳ 2 i + h2 i (43) 12 n E(θ i )α(θ i )h i (44) i=1 h/2 M T = B y E(y)α(y)dy = B h/2 i=1 n E(θ i )α(θ i )h i ȳ i (45) i=1 (46) Here E(θ i ), α(θ i ), h i, and ȳ i are the xdirection modulus, xdirection thermal expansion coefficient, thickness, and midpoint of ply i with orientation angle θ i. A 11, B 11, and D 11 are the (1, 1) elements of the usual laminated plate theory A, B, and D matrices except for the extra factor of B because F and M are total forces and moments instead of force and moment resultants. By the usual rules for rotation of thermomechanical properties, E(θ i ) and α(θ i ) are 1 E(θ i ) ( = cos4 θ i 1 + 2ν ) 12 sin 2 θ i cos 2 θ i + sin4 θ i (47) E 1 G 12 E 1 E 2 α(θ i ) = α 1 cos 2 θ i + α 2 sin 2 θ i (48) Here E 1, E 2, G 12, ν 12, α 1, and α 2 are the inplane tensile and shear moduli, Poisson s ratio, and thermal expansion coefficients of the ply material with 1 being the fiber direction and 2 being the transverse direction. Finally, setting F = 0 and solving for κ gives where the effective beam properties are κ = C κm + α κ T (49) A 11 Cκ = A 11 D 11 B11 2 and α κ = B 11N T A 11 M T A 11 D 11 B 2 11 (50) References [1] Ripling, E. J., S. Mostovoy, and R. L. Patrick Materials Research & Standards 1964, 4, [2] Mostovoy, S. and E. J. Ripling J. Appl. Polym. Sci. 1966, 10, [3] Mostovoy, S. and E. J. Ripling J. Appl. Polymer Sci. 1971, 15, [4] ASTM D , in Annual Book of ASTM Standards 1996, 15.06, [5] ASTM D a, in Annual Book of ASTM Standards 1996, 15.03, [6] Reeder, J. R. and J. H. Crews, Jr. AIAA J. 1990, 28, [7] Hashemi, S., A. J. Kinloch, and J. G. Williams Proc. R. Soc. Lond. 1990, A347, [8] Blackman, B., A. J. Kinloch, and J. G. Williams, personal communication. [9] Williams, J. G. J. Comp. Mater. 1987, 21, [10] Williams, J. G. in Proc. Int l Mechanical Engineering Congress and Exhibition: The Winter Annual Meeting of the ASME, Symposium on Mechanics of Plastics and Plastic Composites November 1995, San Francisco, USA. [11] Williams, J. G. Comp. Sci. & Tech. 1989, 35,
16 74 J. A. Nairn / International Journal of Adhesion & Adhesives 20 (1999) [12] Nairn, J. A. J. Applied Mech. 1997, 64, [13] Crandall, S. H., N. C. Dahl, and T. J. Lardner, An Introduction to the Mechanics of Solids, McGraw Hill Book Company, New York (1978). [14] Timoshenko, S. J. Opt. Soc. Amer. 1925, 11, [15] Krishnamurthy, T., Ramamurthy, T. S., Vijayakumar, K. and Dattaguru, B. in Proc. Int. Conf. Finite Elements in Computational Mechanics, 26 December 1985, Bombay, India, [16] Kanninen, M. F. Int. J. Fract. 1973, 9, [17] Nairn, J. A. and P. Zoller ASTM STP , [18] Hudson, R. C., B. D. Davidson, and J. J. Polaha Proc. ICCM , I, [19] Polaha, J. J., B. D. Davidson, R. C. Hudson, and A. Pieracci J. Reinforced Plast. and Comp. 1996, 15, [20] Hunston, D. L. Comp. Tech. Rev. 1984, 6, [21] Hunston, D. L., R. J. Moulton, N. J. Johnston, and W. D. Bascom in Toughened Composites, ed. N. J. Johnston 1987, ASTM STP 937, [22] Liu, S. and J. A. Nairn J. Reinf. Plast. & Comp. 1992, 11, [23] Davies, P., W. Cantwell, C. Moulin, and H. H. Kausch Comp. Sci. & Tech. 1989, 36,
FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES
Advanced Composite Letters, Vol. 9, No. 6, 373383 000 Full Article ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES John A. Nairn Material
More informationMixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES
MixedMode Fracture Toughness Determination USING NONCONVENTIONAL TECHNIQUES IDMEC Pólo FEUP DEMec  FEUP ESM Virginia Tech motivation fracture modes conventional tests [mode I] conventional tests [mode
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationOn the calculation of energy release rates for cracked laminates with residual stresses
International Journal of Fracture, 39, 67 93 006) On the calculation of energy release rates for cracked laminates with residual stresses J. A. NAIRN Wood Science and Engineering, Oregon State University,
More informationFig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double cantilever beam (DCB) specimens.
a). Cohesive Failure b). Interfacial Failure c). Oscillatory Failure d). Alternating Failure Fig. 1. Different locus of failure and crack trajectories observed in mode I testing of adhesively bonded double
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS. Ford Research Laboratory, Ford Motor Company, Dearborn, MI 48121, U.S.A. 1.
TOUGHNESS OF PLASTICALLYDEFORMING ASYMMETRIC JOINTS M. D. Thouless, M. S. Kafkalidis, S. M. Ward and Y. Bankowski Department of Mechanical Engineering and Applied Mechanics, University of Michigan, Ann
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationExperimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives
Experimentally Calibrating Cohesive Zone Models for Structural Automotive Adhesives Mark Oliver October 19, 2016 Adhesives and Sealants Council Fall Convention contact@veryst.com www.veryst.com Outline
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationMaterials and Structures
Journal of Mechanics of Materials and Structures BRITTLE FRACTURE BEYOND THE STRESS INTENSITY FACTOR C. T. Sun and Haiyang Qian Volume 4, Nº 4 April 2009 mathematical sciences publishers JOURNAL OF MECHANICS
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT INTERFACES, AND TRACTIONLOADED CRACKS
Composites Science and Technology, 61, 159167 (000) c 000 Elsevier Science Limited Author Prepared Preprint. All rights reserved ELSEVIER FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT
More informationFracture Mechanics Analysis of Composite Microcracking: Experimental Results in Fatigue
Proceedings of the 5 th Technical Conference on Composite Materials, American Society of Composites, East Lansing, Michigan, June 1114, 1990). Fracture Mechanics Analysis of Composite Microcracking: Experimental
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE
ID1274 SPLIT ANGLEPLY BEAM SPECIMEN FOR MEASUREMENT OF FRACTURE TOUGHNESS WITH MODE III STRESS STATE Kunigal Shivakumar, Srikant Ghantae * and Matthew Sharpe Center for Composite Materials Research North
More informationINFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK BETWEEN THE TWO LAYERS
Djoković, J. M., et.al.: Influence of Temperature on Behavior of the Interfacial THERMAL SCIENCE: Year 010, Vol. 14, Suppl., pp. S59S68 S59 INFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK
More informationNASA TECHNICAL MEMORANDUM
NASA TECHNICAL MEMORANDUM 102777 NONLINEAR ANANLYSIS AND REDESIGN OF THE MIXEDMODE BENDING DELAMINATION TEST J. R. Reeder and J. H. Crews, Jr. January 1991 National Aeronautics and Space Administration
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationNONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM
Engineering MECHANICS, Vol., 015, No., p. 95 10 95 NONLINEAR FRACTURE BEHAVIOR OF DOUBLE CANTILEVER BEAM Viktor Rizov* This article describes a theoretical study of nonlinear fracture behavior of the
More informationInt. J. Fracture, 119, 2003, 2546
Int. J. Fracture, 119, 003, 546 THE USE OF A COHESIVE ZONE MODEL TO STUDY THE FRACTURE OF FIBRE COMPOSITES AND ADHESIVELYBONDED JOINTS Blackman, B.R.K., Hadavinia, H., Kinloch, A.J. and Williams, J.G.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationFRACTURE MECHANICS TEST METHODS
DEVELOPMENT AND EVALUATION OF FRACTURE MECHANICS TEST METHODS FOR SANDWICH COMPOSITES Dan Adams Department of Mechanical Engineering University it of Utah Salt Lake City, UT AMTAS A t 2012 M ti AMTAS Autumn
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationLaminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 375 June 1980 Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
More informationBen W. Kim 1 and John A. Nairn 2
J. Materials Science, submitted (2002) Author prepared reprint Experimental Verification of the Effects of Friction and Residual Stress on the Analysis of Interfacial Debonding and Toughness in Single
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationSSRG International Journal of Mechanical Engineering (SSRGIJME) volume1 issue5 September 2014
Finite Element Modeling for Delamination Analysis of Double Cantilever Beam Specimen Mohammed Waseem H.S. 1, Kiran Kumar N. 2 1 Post Graduate Student, 2 Asst. Professor Dept. of Mechanical Engineering,
More informationCHARACTERIZATION OF CURING STRESS EFFECTS ON FRACTURE BEHAVIOUR OF FRP COMPOSITE LAMINATE WITH ELLIPTICAL CUTOUTS
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS CHARACTERIZATION OF CURING STRESS EFFECTS ON FRACTURE BEHAVIOUR OF FRP COMPOSITE LAMINATE WITH ELLIPTICAL CUTOUTS Poosa R Babu, Pradhan B Department
More informationSize effect in the strength of concrete structures
Sādhanā Vol. 27 Part 4 August 2002 pp. 449 459. Printed in India Size effect in the strength of concrete structures B L KARIHALOO and Q Z XIAO Division of Civil Engineering School of Engineering Cardiff
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationStress intensity factor analysis for an interface crack between dissimilar isotropic materials
Stress intensity factor analysis for an interface crack between dissimilar isotropic materials under thermal stress T. Ikeda* & C. T. Sun* I Chemical Engineering Group, Department of Materials Process
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationCOMELD TM JOINTS: A NOVEL TECHNIQUE FOR BONDING COMPOSITES AND METAL
COMELD TM JOINTS: A NOVEL TECHNIQUE FOR BONDING COMPOSITES AND METAL F.J. Guild *, P.J. Hogg + and W. Tu School of Engineering and Materials Science, Queen Mary, University of London, London E1 4NS, UK
More informationLecture 4 Honeycombs Notes, 3.054
HoneycombsInplane behavior Lecture 4 Honeycombs Notes, 3.054 Prismatic cells Polymer, metal, ceramic honeycombs widely available Used for sandwich structure cores, energy absorption, carriers for catalysts
More informationFracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments
Engineering Fracture Mechanics ) 4 Author prepared preprint Fracture mechanics analysis of coating/substrate systems Part I: Analysis of tensile and bending experiments SungRyong Kim a, John A. airn
More informationSCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL
SCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL LAMINATES J. G. Carrillo 1, S. McKown 1, M. Mujib 1 and W. J. Cantwell 1. R. Day 2 1 Department of Engineering, University of Liverpool,
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationMicrocracking, MicrocrackInduced. Delamination, and Longitudinal
NASA Contractor Final Report Microcracking, MicrocrackInduced Delamination, and Longitudinal Splitting of Advanced Composite Structures John A. Nairn University of Utah Salt Lake City, Utah Prepared for
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationComb resonator design (2)
Lecture 6: Comb resonator design () Intro Intro. to Mechanics of Materials School of Electrical l Engineering i and Computer Science, Seoul National University Nano/Micro Systems & Controls Laboratory
More informationDurability of bonded aircraft structure. AMTAS Fall 2016 meeting October 27 th 2016 Seattle, WA
Durability of bonded aircraft structure AMTAS Fall 216 meeting October 27 th 216 Seattle, WA Durability of Bonded Aircraft Structure Motivation and Key Issues: Adhesive bonding is a key path towards reduced
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationEXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS
Gépészet 008 Budapest, 90.May 008. G008J04 EXPERIMENTBASED CRITERION FOR THE CRACK STABILITY ANALYSIS IN COMPOSITE MATERIALS András Szekrényes Assistant Professor, Department of Applied Mechanics,
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationKeywords: Adhesively bonded joint, laminates, CFRP, stacking sequence
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS GLOBAL AND LOCAL INFLUENCE OF STACKING SEQUENCE ON THE STRENGTH OF ADHESIVELY BONDED JOINTS OF CFRP LAMINATES J. Rousseau*, P. Satthamnuwong DRIVE,
More informationStrength and Damage Tolerance of Adhesively Bonded Joints: StressBased and FractureBased Approaches
Strength and Damage Tolerance of Adhesively Bonded Joints: StressBased and FractureBased Approaches Hyonny Kim Assistant Professor School of Aeronautics and Astronautics, Purdue University presented
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationA PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS
1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams
More informationDerivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis
Derivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis S. Quinn, S. Sambasivam and J.M. DulieuBarton School of Engineering Sciences, University of Southampton,
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationAnalytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal stresses
International Journal of Adhesion & Adhesives 19 (1999) 59 7 Analytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationDYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS
DYNAMIC DELAMINATION OF AERONAUTIC STRUCTURAL COMPOSITES BY USING COHESIVE FINITE ELEMENTS M. Ilyas, F. Lachaud 1, Ch. Espinosa and M. Salaün Université de Toulouse, ISAE/DMSM, 1 avenue Edouard Belin,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationEFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION
EFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION J.Varna and R.Joffe Dept of Applied Physics and Mechanical Engineering Lulea University of Technology, SE 97187, Lulea,
More informationFinite Element and Plate Theory Modeling of Acoustic Emission Waveforms. NASA Langley Research Center. Hampton, VA *University of Denver
Finite Element and Plate Theory Modeling of Acoustic Emission Waveforms W. H. Prosser, M. A. Hamstad + *, J. Gary +, and A. O Gallagher + NASA Langley Research Center Hampton, VA 236811 *University of
More informationEvaluation Axisymmetric Analysis of Thermal Stress Residual Near Fiber/Epoxy Interface
Materials Research, Vol. 12, No. 2, 133137, 2009 2009 Evaluation Axisymmetric Analysis of Thermal Stress Residual Near Fiber/Epoxy Interface Aboubakar Seddik Bouchikhi Department of Mechanical Engineering,
More informationFracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach Ludovic Noels Computational & Multiscale Mechanics of
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationTESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING.
TESTING AND ANALYSIS OF COMPOSITE SKIN/STRINGER DEBONDING UNDER MULTIAXIAL LOADING. Ronald Krueger*, Michael K. Cvitkovich*, T. Kevin O'Brien**, and Pierre J. Minguet*** * National Research Council Research
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationA FINITE ELEMENT STUDY OF ELASTICPLASTIC HEMISPHERICAL CONTACT BEHAVIOR AGAINST A RIGID FLAT UNDER VARYING MODULUS OF ELASTICITY AND SPHERE RADIUS
Proceedings of the International Conference on Mechanical Engineering 2009 (ICME2009) 2628 December 2009, Dhaka, Bangladesh ICME09 A FINITE ELEMENT STUDY OF ELASTICPLASTIC HEMISPHERICAL CONTACT BEHAVIOR
More informationFRACTURE MECHANICS IN ANSYS R16. Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model
FRACTURE MECHANICS IN ANSYS R16 Session 04 Fracture Mechanics using Cohesive Zone Material (CZM) Model COHESIVE ZONE MATERIAL MODEL (CZM) Fracture or delamination along an interface between phases plays
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationTentamen/Examination TMHL61
Avd Hållfasthetslära, IKP, Linköpings Universitet Tentamen/Examination TMHL61 Tentamen i Skademekanik och livslängdsanalys TMHL61 lördagen den 14/10 2000, kl 812 Solid Mechanics, IKP, Linköping University
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More information